# Modeling Electrolytically Top-Gated Graphene

- First Online:

- Received:
- Accepted:

**Part of the following topical collections:**

## Abstract

We investigate doping of a single-layer graphene in the presence of electrolytic top gating. The interfacial phenomenon is modeled using a modified Poisson–Boltzmann equation for an aqueous solution of simple salt. We demonstrate both the sensitivity of graphene’s doping levels to the salt concentration and the importance of quantum capacitance that arises due to the smallness of the Debye screening length in the electrolyte.

### Keywords

Graphene Electrolyte Poisson–Boltzmann model Gating Quantum capacitance## Introduction

Carbon nano-structures show great promise in many applications, including chemical and biological sensors. While carbon nanotubes (CNTs) have been extensively studied in that context for quite some time [1, 2], investigations of graphene as a sensor are only beginning to appear [3, 4, 5]. Sensory function of carbon nano-structures is generally implemented in the configuration of a field effect transistor (FET), with a prominent role played by the gate potential that controls the current through the device. Biochemical applications require good understanding of the interaction of carbon nano-structures with aqueous solutions [5], often in the context of the electrochemical top gating [6]. While significant progress has been achieved in understanding the interaction of CNT–FETs with the electrolytic environment [7, 8, 9], similar studies involving graphene have appeared only very recently [6], focusing on the screening effect of an ion solution on charge transport through graphene-based FETs [10], as well as on the measurement of the quantum capacitance of graphene as an ultimately thin electrode in an aqueous solution [11].

The top gating of a graphene-based FET with a solid or liquid electrolyte presents several advantages compared to the conventional back gating with a metallic electrode. Upon application of gate voltage, free ions in the electrolyte re-distribute themselves, forming an electrostatic double layer (EDL) at the interface between graphene and the electrolytic solution [12]. Depending on the ion concentration, the EDL can be only a few nanometers thick, while still providing efficient shielding of graphene. As a consequence, the capacitance of the EDL in an electrolyte can be much higher than the capacitance of the back gate, which is typically separated from graphene with a layer of SiO_{2} a few hundred nanometers thick [12]. This property of the EDL enables a much better control of the surface potential on the graphene layer, while requiring a much lower operating voltage that needs to be applied to the reference electrode in the electrolyte than voltages currently used with back gates [12]. The applied voltage then modifies the chemical potential of graphene, resulting in changes in its observable properties such as conductance. Since properties of the EDL depend on the ion concentration, monitoring the resulting changes in graphene’s conductance can provide a means for sensor application, e.g., in measuring the amount of salt in the solution.

On the other hand, referring to the electrical model of the electrolytic gating as a series connection of capacitors [13], the high gate capacitance in the electrolyte gives a much more prominent role to the quantum capacitance of graphene than does the back gate [11, 14, 15, 16]. In addition, doping levels of an electrolytically top-gated graphene have been reported recently [6] to be much higher than those obtained with the conventional back gate [17]. At the same time, mobile ions in the solution seem to provide a much more effective screening of charged impurities underneath the graphene, thereby significantly increasing the charge carrier mobility in graphene in comparison with some other high-κ dielectric environments [18]. All these facts indicate that electrolytic top gating provides a means to develop high-performance FETs.

While the above few experimental observations reveal quite fascinating aspects of the graphene–electrolyte interaction, theoretical modeling of this system seems to be lagging behind the experiment. It is therefore desirable and tempting to discuss doping of a single layer of graphene by a remote gate electrode immersed in a thick layer of electrolyte by using two simple models: one describing graphene’s π electron band structure in the linear energy dispersion approximation [12], and the other describing the distribution of ions in the electrolyte by a one-dimensional (1D) Poisson–Boltzmann (PB) model, which takes advantage of the planar symmetry of the problem [13]. However, it should be emphasized that the experiments involving electrolytic top gating of both CNTs [7, 8] and graphene [6, 10] use rather high voltages, on the order of 1–2 V, which can cause significant crowding of counter-ions at the electrolyte–graphene interface. It is therefore necessary to go beyond the standard PB model by taking into account the steric effects, i.e., the effects of finite size of ions in the solution. To that aim, we shall use the modified Poisson–Boltzmann (mPB) model developed by Borukhov et al. [22, 23], which retains analytical tractability of the original 1D-PB model. In addition, applied voltages beyond 1 V also require taking into account non-linearity of graphene’s band energy dispersion, giving small but noticeable corrections to the linear approximation.

We shall consider here a simple 1:1 electrolyte representing an aqueous solution of NaF because both the Na^{+} and the *F*^{−} ions are chemically inert allowing us to neglect their specific adsorption on the graphene surface [10, 13]. In particular, we shall analyze the density of doped charge carriers in graphene at room temperature (RT) as a function of both the applied voltage and the salt concentration to elucidate graphene’s sensor ability. In addition, we shall evaluate the contributions of both the graphene and the EDL in the total gate capacitance in terms of the applied voltage to reveal the significance of quantum capacitance, as well as to elucidate the behavior of the EDL under high voltages. We shall cover broad ranges of both the salt concentration, going from μM to a physiologically relevant value, and the applied voltage, going up to about 2 V.

After outlining our theoretical models for graphene and the EDL in the next section, we shall introduce several reduced quantities of relevance for these two vastly different systems and present our results in the following section. Finally, conclusion follows. Note that we shall use gaussian units (4πε_{0} = 1) throughout the paper, unless otherwise explicitly stated.

## Theoretical Model

*g*

_{d}= 4 is the spin and the band valley degeneracy factor, and

*v*

_{F}≈

*c*/300 is the Fermi speed of graphene, with

*c*being the speed of light in vacuum [12]. In the intrinsic, or undoped graphene, the Fermi energy level sits precisely at the neutrality point, ɛ

_{F}= 0, also called the Dirac point. Therefore, the electrical conductivity of graphene is easily controlled, e.g., by applying a gate voltage

*V*

_{A}that will cause doping of graphene’s π bands with electrons or holes (depending on the sign of

*V*

_{A}), which can attain the number density per unit area,

*n*, with a typical range of

*n*∼ 10

^{11}–10

^{13}cm

^{−2}[12]. In a doped graphene, Fermi level moves to Open image in new window, where sgn(

*n*) = ± 1 for electron (hole) doping. At a finite temperature

*T*, one can express the charge carrier density in a doped graphene in terms of its chemical potential μ as [19]

where Open image in new window with *k*_{B} being the Boltzmann constant. We shall use in our calculations a full, non-linear expression for the π electron band density, ρ(ɛ), given in Eq. 14 of Ref. [12]. However, for the sake of transparency, the theoretical model for graphene will be outlined below within the linear density approximation, ρ(ɛ) ≈ ρ_{L} (ɛ). We note that this approximation is accurate enough for low to moderate doping levels, such that, e.g., Open image in new window, and it only incurs a relative error of up to a few percent when Open image in new window.

*V*

_{Q}= −μ/

*e*, where

*e*> 0 is the proton charge, which is associated with the quantum-mechanical effects of graphene’s band structure [20], and relate it to the induced charge density per unit area on doped graphene, σ = −

*en*, via the Eq. 1,

*C*

_{Q}= dσ/d

*V*

_{Q}, to obtain from Eq. 2 the quantum capacitance of a single layer of graphene as [14]

with the value of λ_{Q} ≈ 18 nm at RT. Note from Eq. 3 that graphene’s quantum capacitance grows practically linearly with *V*_{Q} when this potential exceeds the thermal potential, *V*_{th} = 1/(*e* β), having the value of ≈26 mV at RT.

*z*:

*z*electrolyte containing the bulk number density per unit volume,

*N*, of dissolved salt ions. Taking advantage of planar symmetry, we place an

*x*axis perpendicular to graphene and pointing into the electrolyte. The theory developed by Borukhov et al. [22, 23] to model finite ion size uses the mPB equation for the electrostatic potential

*V*(

*x*) in the electrolyte at a distance

*x*from graphene, given by

*z*(=1) is the valency of ions, ε is relative dielectric constant of water (≈80, assumed to be constant throughout the electrolyte), and γ = 2

*a*

^{3}

*N*is the packing parameter of the solvated ions, which are assumed to have same effective size, equal to

*a*[22, 23]. We note that the standard PB model is recovered from Eq. 5 in the limit γ → 0 [13]. By assuming the boundary condition

*V*(

*x*) = 0 (and hence d

*V*/d

*x*= 0) at

*x*→ ∞, deep into the electrolyte bulk, Eq. 5 can be integrated once giving a relation between the electric field and the potential at a distance

*x*from graphene. Assuming that graphene is placed at

*x*= 0, one can use the boundary condition at the distance

*d*of closest approach for ions in the electrolyte to graphene,

*V*

_{D}=

*V*(

*d*), across the EDL as

*V*

_{A}, applied between the reference electrode in the electrolyte and graphene can be written as

where *V*_{pzc} = (*W*_{gr} − *W*_{ref})/*e* is the potential of zero charge [13] that stems from difference between the work functions of graphene and the reference electrode, *W*_{gr} and *W*_{ref}, respectively, and *V*_{cl} = 4πhσ/ε′ is the potential drop across a charge-free region between the compact layer of the electrolyte ions condensed on the graphene surface, having the thickness *h* on the order of the distance of closest approach *d*[23, 24], and with ε′ < ε taking into account a reduction of the dielectric constant of water close to a charged wall [25]. In our calculations, we shall neglect these two contributions to the applied potential in Eq. 8 because *V*_{pzc} merely shifts the zero of that potential, while a proper modeling of *V*_{cl} involves large uncertainty [23, 24]. However, usually the effects of *V*_{cl} can be considered either small [23] or incorporated in the mPB model via saturation of the ion density at the electrolyte–graphene interface for high potential values [22]. Consequently, *V*_{D} and *V*_{Q} represent the two main contributions in Eq. 8, with *V*_{D} being the surface potential of graphene that shifts its Dirac point, and *V*_{Q} being responsible for controlling the doping of graphene by changing its chemical potential. Finally, we note that all results of our calculations will be symmetrical relative to the change in sign of the applied potential because of our assumption that the effective sizes of the positive and negative ions are equal [22, 23], but this constraint can be lifted by a relatively simple amendment to the mPB model [24].

*V*

_{A}=

*V*

_{Q}+

*V*

_{D}, we obtain the total differential capacitance of the electrolytically top-gated graphene as

*C*

_{Q}(

*V*

_{Q}) is given in Eq. 3, and

*C*

_{D}(

*V*

_{D}) = dσ/d

*V*

_{D}is the differential capacitance per unit area of the EDL, which can be obtained from Eq. 7as [23, 24],

*V*

_{D}, and hence for low density of ions at the graphene–EDL interface, one can set γ → 0 in Eq. 10 to recover an expression for the EDL capacitance in the standard PB model [13],

We further note that, while Eq. 11 implies an unbounded growth of the EDL capacitance with *V*_{D} in the PB model, Eq. 10 suggests a non-monotonous behavior that will eventually give rise to a saturation of the total gate capacitance at high applied voltages.

## Results

*V*

_{th}= 1/(

*e*β), all potentials can be written asOpen image in new window. While typical regimes of graphene doping require onlyOpen image in new window, we shall extend this range in our calculations up to aboutOpen image in new windowto represent doping levels in recent experiments in electrolytic environment [6]. Next, referring to Eq. 2, we define the characteristic number density of doped charge carriers in graphene by Open image in new window, which has the value of

*n*

_{0}≈ 10

^{11}cm

^{−2}at RT. Therefore, defining the reduced density by Open image in new window, and hence Open image in new window, we note that Open image in new window may reach up to around 10

^{3}[6, 12]. It is worthwhile mentioning that graphene’s characteristic parameters λ

_{Q}and

*n*

_{0}are related via ελ

_{B}λ

_{Q}

*n*

_{0}= 1, where λ

_{B}= β

*e*

^{2}/ε is the Bjerrum length of the aqueous environment, taking the value of λ

_{B}≈ 0.7 nm at RT [13]. Furthermore, it follows from Eq. 3 that the natural unit of capacitance for this system is

*C*

_{0}=

*en*

_{0}/

*V*

_{th}= λ

_{Q}

^{−1}, taking the value of

*C*

_{0}≈ 0.6 μF/cm

^{2}at RT. Turning now to Eq. 7, one can define the characteristic number density of ions per unit volume in the solution by

*N*

_{0}≈ 1.08 × 10

^{−6}nm

^{−3}≈ 1.8 μM at RT. Defining the reduced concentration of ions in the bulk of the electrolyte by Open image in new window, it would be of interest to explore a broad range of its values, e.g., Open image in new window. Finally, in order to estimate the packing parameter, we write Open image in new window and take

*a*= λ

_{B}to obtain ν = 2λ

_{B}

^{3}

*N*

_{0}≈ 7 × 10

^{−7}. With these definitions, Eqs. 2 and 7 now read, respectively,

*n*≈ 10

^{11}cm

^{−2}[26, 27]. Therefore, it seems that Open image in new window would be an optimal range of applied voltages for sensor applications of the electrolytically top-gated graphene in probing salt concentrations in the sub-millimole range.

*C*, we note that the reduced capacitances,Open image in new windowandOpen image in new window, are obtained from Eqs. 3and10as

showing thatOpen image in new windowandOpen image in new windoware comparable in magnitude for vanishing potentials when the salt concentration isOpen image in new window. Moreover, referring to Eq. 9as an electrical model where graphene and the EDL act as a series connection of capacitors, it follows that graphene’s quantum capacitance *C*_{Q} will be promoted as the dominant contribution to the total gate capacitance as the salt concentration increases.

^{5}(corresponding to

*N*≈ 1.8 μM and 0.18 M, respectively). We show our results for the reduced applied voltages up toOpen image in new windowin order to elucidate the effect of saturation in the total capacitance that occurs atOpen image in new window(corresponding to

*V*

_{A}≈ 2.21 V) forOpen image in new windowand atOpen image in new window(corresponding to

*V*

_{A}≈ 1.95 V) forOpen image in new window. As can be seen from dotted curves in Fig. 3, showing a non-monotonous dependence of the EDL capacitance on the applied voltage, the saturation effect in the total capacitance of the electrolytically top-gated graphene is a consequence of the steric effect of the electrolyte ions that are crowded at the graphene surface at high applied voltages [23]. Even though the voltages where the saturation occurs are relatively high, they may still be accessible in experiments on graphene. Furthermore, we see in Fig. 3 that at intermediate applied voltages, the rate of change of the total capacitance follows closely that of the quantum capacitance, with the value ≈23 μF/(V cm

^{2}) that is commensurate with recent measurement [11]. At the lowest applied voltages, one notices in Fig. 3 a “rounding” of the total capacitance as a function of voltage for low salt concentrations, which comes from the EDL capacitance. Such rounding is observed in the recent experiment [11].

*V*

_{A}splits between the potential drop

*V*

_{D}across the EDL and the voltage

*V*

_{Q}pertaining to the change in graphene’s chemical potential. We therefore display in Fig. 4 the variation of the fraction

*r*=

*V*

_{D}/

*V*

_{A}as a function of the reduced salt concentration in the electrolyteOpen image in new windowfor several values of the applied voltage

*V*

_{A}. One can see that at low salt concentrations, the potentials

*V*

_{Q}and

*V*

_{D}are roughly comparable in magnitude, although the ratio

*r*increases in favor of the potential drop across the electrolyte as the applied voltage increases. However, this trend is reversed at high salt concentrations and, more importantly, Fig. 4 shows that the most of the applied voltage is used to increase graphene’s chemical potential for a full range of applied voltages when salt concentration

*N*exceeds, say, mM. Besides its importance for applications, the fact that the potential drop across the electrolyte remains very small at high applied voltages also alleviates concern that a high electric field in the electrolyte may cause the onset of voltage-dependent electrochemical reactions on graphene.

## Concluding Remarks

We have analyzed the doping of single-layer graphene due to application of the gate potential through an aqueous solution of salt using a modified Poisson–Boltzman model for electrolyte and found great sensitivity of the induced charge density in graphene to the broad ranges of both salt concentration and applied voltage. We have further analyzed differential capacitance of the electrolytically top-gated graphene and found that its quantum capacitance is promoted as the dominant component owing to a reduction in the Debye length of the electric double layer when the salt concentration increases. In this case, very little potential drop appears across the electrolyte, and graphene takes most of the voltage drop to shift its chemical potential. These findings have several important consequences.

First, since graphene’s conductivity is dependent upon its chemical potential, its sensitivity to the salt concentration implies good prospects for applications in biochemical sensors, especially for in vivo electrochemical measurements in biological systems owing to graphene’s natural bio-compatibility. Next, since most of the applied voltage can be used to increase the chemical potential of graphene, as opposed to a potential drop across the electrolyte, one can envision ways to use a very thin top gate (in the form of a liquid or solid electrolyte) that requires relatively low gate voltage to change the chemical potential (and hence conductivity) of graphene in future small scale field effect devices with tunable conductivity. Among other aspects of the increased role of graphene’s quantum capacitance is reduction of the electrical field across the electrolyte. This can help reduce the rates of voltage-induced electrochemical reactions on graphene’s surface, as well as improve the mobility of charge carriers in graphene by reducing their scattering rates on various impurities. Moreover, since quantum capacitance is basically the capacitance associated with change in carrier densities, it can be seen as analogous to the junction capacitance, and the smaller quantum capacitance could in turn lead to faster switching time for graphene-based devices.

Many of these advantages of top gating through an electrolyte are related to a high bulk dielectric constant of the electrolyte, especially in aqueous solutions. So, even though the oxide thickness can be reduced down to around 2 nm in the present generation conventional MOS structures, the much higher dielectric constant of water in comparison with SiO_{2} should provide for a higher gate capacitance, translating into much better field effect performance, as discussed above. However, dielectric constant of an electrolyte can be significantly reduced close to a charged surface [24, 25], and this issue has yet to be discussed in the context of electrolytic top gating of carbon nano-structures.

## Notes

### Acknowledgments

This work was supported by the Natural Sciences and Engineering Research Council of Canada.

**Open Access**

This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.

### References

- 1.Kong J, Franklin NR, Zhou CW, Chapline MG, Peng S, Cho KJ, Dai HJ:
**Nanotube molecular wires as chemical sensors.***Science*2000,**287:**622. COI number [1:CAS:528:DC%2BD3cXovVWgtA%3D%3D]; Bibcode number [2000Sci...287..622K] COI number [1:CAS:528:DC%2BD3cXovVWgtA%3D%3D]; Bibcode number [2000Sci...287..622K] 10.1126/science.287.5453.622CrossRefGoogle Scholar - 2.Kauffman DR, Star A:
**Electronically monitoring biological interactions with carbon nanotube field-effect transistors.***Chem. Soc. Rev.*2008,**37:**1197. COI number [1:CAS:528:DC%2BD1cXmtlSisb4%3D] COI number [1:CAS:528:DC%2BD1cXmtlSisb4%3D] 10.1039/b709567hCrossRefGoogle Scholar - 3.Schedin F, Geim AK, Morozov SV, Hill EW, Blake P, Katsnelson MI, Novoselov KS:
**Detection of individual gas molecules adsorbed on graphene.***Nat. Mater.*2007,**6:**652. COI number [1:CAS:528:DC%2BD2sXpvFKjsrs%3D]; Bibcode number [2007NatMa...6..652S] COI number [1:CAS:528:DC%2BD2sXpvFKjsrs%3D]; Bibcode number [2007NatMa...6..652S] 10.1038/nmat1967CrossRefGoogle Scholar - 4.Robinson JT, Perkins FK, Snow ES, Wei ZQ, Sheehan PE:
**Reduced graphene oxide molecular sensors.***Nano Lett.*2008,**8:**3137. COI number [1:CAS:528:DC%2BD1cXhtVOhtL3M]; Bibcode number [2008NanoL...8.3137R] COI number [1:CAS:528:DC%2BD1cXhtVOhtL3M]; Bibcode number [2008NanoL...8.3137R] 10.1021/nl8013007CrossRefGoogle Scholar - 5.Ang PK, Chen W, Wee ATS, Loh KP:
**Solution-gated epitaxial graphene as pH sensor.***J. Am. Chem. Soc.*2008,**130:**14392. COI number [1:CAS:528:DC%2BD1cXht1ertb%2FL] COI number [1:CAS:528:DC%2BD1cXht1ertb%2FL] 10.1021/ja805090zCrossRefGoogle Scholar - 6.Das A, Pisana S, Chakraborty B, Piscanec S, Saha SK, Waghmare UV, Novoselov KS, Krishnamurthy HR, Geim AK, Ferrari AC, Sood AK:
**Monitoring dopants by Raman scattering in an electrochemically top-gated graphene transistor.***Nat. Nanotechnol.*2008,**3:**210. COI number [1:CAS:528:DC%2BD1cXkt1Slu74%3D] COI number [1:CAS:528:DC%2BD1cXkt1Slu74%3D] 10.1038/nnano.2008.67CrossRefGoogle Scholar - 7.Kruger M, Buitelaar MR, Nussbaumer T, Schonenberger C, Forro L:
**Electrochemical carbon nanotube field-effect transistor.***Appl. Phys. Lett.*2001,**78:**1291. COI number [1:CAS:528:DC%2BD3MXhtl2nsrY%3D]; Bibcode number [2001ApPhL..78.1291K] COI number [1:CAS:528:DC%2BD3MXhtl2nsrY%3D]; Bibcode number [2001ApPhL..78.1291K] 10.1063/1.1350427CrossRefGoogle Scholar - 8.Rosenblatt S, Yaish Y, Park J, Gore J, Sazonova V, McEuen PL:
**High performance electrolyte gated carbon nanotube transistors.***Nano Lett.*2002,**2:**869. COI number [1:CAS:528:DC%2BD38XlsFals7Y%3D]; Bibcode number [2002NanoL...2..869R] COI number [1:CAS:528:DC%2BD38XlsFals7Y%3D]; Bibcode number [2002NanoL...2..869R] 10.1021/nl025639aCrossRefGoogle Scholar - 9.Heller I, Kong J, Williams KA, Dekker C, Lemay SG:
**Electrochemistry at single-walled carbon nanotubes: the role of band structure and quantum capacitance.***J. Am. Chem. Soc.*2006,**128:**7353. COI number [1:CAS:528:DC%2BD28XksFKlur0%3D] COI number [1:CAS:528:DC%2BD28XksFKlur0%3D] 10.1021/ja061212kCrossRefGoogle Scholar - 10.Chen F, Xia JL, Tao NJ:
**Ionic screening of charged-impurity scattering in graphene.***Nano Lett.*2009,**9:**1621. COI number [1:CAS:528:DC%2BD1MXjsFWmtbs%3D]; Bibcode number [2009NanoL...9.1621C] COI number [1:CAS:528:DC%2BD1MXjsFWmtbs%3D]; Bibcode number [2009NanoL...9.1621C] 10.1021/nl803922mCrossRefGoogle Scholar - 11.Xia JL, Chen F, Li JH, Tao NJ:
**Measurement of the quantum capacitance of graphene.***Nat. Nanotechnol.*2009,**4:**505. COI number [1:CAS:528:DC%2BD1MXpsFSisbs%3D]; Bibcode number [2009NatNa...4..505X] COI number [1:CAS:528:DC%2BD1MXpsFSisbs%3D]; Bibcode number [2009NatNa...4..505X] 10.1038/nnano.2009.177CrossRefGoogle Scholar - 12.Castro Neto AH, Guinea F, Peres NM, Novoselov KS, Geim AL:
**The electronic properties of graphene.***Rev. Mod. Phys.*2009,**81:**109. COI number [1:CAS:528:DC%2BD1MXksVamsLY%3D]; Bibcode number [2009RvMP...81..109C] COI number [1:CAS:528:DC%2BD1MXksVamsLY%3D]; Bibcode number [2009RvMP...81..109C] 10.1103/RevModPhys.81.109CrossRefGoogle Scholar - 13.Bard AJ, Faulkner LR:
*Electrochemical Methods: Fundamentals and Applications*. Willey, New York; 2001.Google Scholar - 14.Fang T, Konar A, Xing HL, Jena D:
**Carrier statistics and quantum capacitance of graphene sheets and ribbons.***Appl. Phys. Lett.*2007,**91:**092109. Bibcode number [2007ApPhL..91i2109F] Bibcode number [2007ApPhL..91i2109F] 10.1063/1.2776887CrossRefGoogle Scholar - 15.Guo J, Yoon Y, Ouyang Y:
**Gate electrostatics and quantum capacitance of graphene nanoribbons.***Nano Lett.*2007,**7:**1935. COI number [1:CAS:528:DC%2BD2sXmtFSnur4%3D]; Bibcode number [2007NanoL...7.1935G] COI number [1:CAS:528:DC%2BD2sXmtFSnur4%3D]; Bibcode number [2007NanoL...7.1935G] 10.1021/nl0706190CrossRefGoogle Scholar - 16.Giannazzo F, Sonde S, Raineri V, Rimini E:
**Screening length and quantum capacitance in graphene by scanning probe microscopy.***Nano Lett.*2009,**9:**23. COI number [1:CAS:528:DC%2BD1cXhsVOnsLzI]; Bibcode number [2009NanoL...9...23G] COI number [1:CAS:528:DC%2BD1cXhsVOnsLzI]; Bibcode number [2009NanoL...9...23G] 10.1021/nl801823nCrossRefGoogle Scholar - 17.Sonde S, Giannazzo F, Raineri V, Rimini E:
**Dielectric thickness dependence of capacitive behavior in graphene deposited on silicon dioxide.***J. Vac. Sci. Technol. B*2009,**27:**868. COI number [1:CAS:528:DC%2BD1MXktV2murw%3D] COI number [1:CAS:528:DC%2BD1MXktV2murw%3D] 10.1116/1.3081890CrossRefGoogle Scholar - 18.Ponomarenko LA, Yang R, Mohiuddin TM, Katsnelson MI, Novoselov KS, Morozov SV, Zhukov AA, Schedin F, Hill EW, Geim AK:
**Effect of a high-kappa environment on charge carrier mobility in graphene.***Phys. Rev. Lett.*2009,**102:**206603. COI number [1:STN:280:DC%2BD1MvhtlCntQ%3D%3D]; Bibcode number [2009PhRvL.102t6603P] COI number [1:STN:280:DC%2BD1MvhtlCntQ%3D%3D]; Bibcode number [2009PhRvL.102t6603P] 10.1103/PhysRevLett.102.206603CrossRefGoogle Scholar - 19.Radovic I, Hadzievski Lj, Miskovic ZL:
**Polarization of supported graphene by slowly moving charges.***Phys. Rev. B*2008,**77:**075428. Bibcode number [2008PhRvB..77g5428R] Bibcode number [2008PhRvB..77g5428R] 10.1103/PhysRevB.77.075428CrossRefGoogle Scholar - 20.Fernandez-Rossier J, Palacios JJ, Brey L:
**Electronic structure of gated graphene and graphene ribbons.***Phys. Rev. B*2007,**75:**205441. Bibcode number [2007PhRvB..75t5441F] Bibcode number [2007PhRvB..75t5441F] 10.1103/PhysRevB.75.205441CrossRefGoogle Scholar - 21.Abramowitz M, Stegun IA:
*Handbook of Mathematical Functions*. National Bureau of Standards, Washington, DC; 1965.Google Scholar - 22.Borukhov I, Andelman D, Orland H:
**Steric effects in electrolytes: a modified Poisson–Boltzmann equation.***Phys. Rev. Lett.*1997,**79:**435. COI number [1:CAS:528:DyaK2sXkvFGmsrs%3D]; Bibcode number [1997PhRvL..79..435B] COI number [1:CAS:528:DyaK2sXkvFGmsrs%3D]; Bibcode number [1997PhRvL..79..435B] 10.1103/PhysRevLett.79.435CrossRefGoogle Scholar - 23.Kilic MS, Bazant MZ, Ajdari A:
**Steric effects in the dynamics of electrolytes at large applied voltages. I. Double-layer charging.***Phys. Rev. E*2007,**75:**021502. Bibcode number [2007PhRvE..75b1502K] Bibcode number [2007PhRvE..75b1502K] 10.1103/PhysRevE.75.021502CrossRefGoogle Scholar - 24.Kornyshev AA:
**Double-layer in ionic liquids: paradigm change.***J. Phys. Chem B*2007,**111:**5545. COI number [1:CAS:528:DC%2BD2sXkslaru78%3D] COI number [1:CAS:528:DC%2BD2sXkslaru78%3D] 10.1021/jp067857oCrossRefGoogle Scholar - 25.Abrashkin A, Andelman D, Orland H:
**Dipolar Poisson–Boltzmann equation: ions and dipoles close to charge interfaces.***Phys. Rev. Lett.*2007,**99:**077801. Bibcode number [2007PhRvL..99g7801A] Bibcode number [2007PhRvL..99g7801A] 10.1103/PhysRevLett.99.077801CrossRefGoogle Scholar - 26.Tan YW, Zhang Y, Bolotin K, Zhao Y, Adam S, Hwang EH, Das Sarma S, Stormer HL, Kim P:
**Measurement of scattering rate and minimum conductivity in graphene.***Phys. Rev. Lett.*2007,**99:**246803. Bibcode number [2007PhRvL..99x6803T] Bibcode number [2007PhRvL..99x6803T] 10.1103/PhysRevLett.99.246803CrossRefGoogle Scholar - 27.Adam S, Hwang EH, Rossi E, Das Sarma S:
**Theory of charged impurity scattering in two-dimensional graphene.***Solid State Commun.*2009,**149:**1072. COI number [1:CAS:528:DC%2BD1MXms1SqsL4%3D]; Bibcode number [2009SSCom.149.1072A] COI number [1:CAS:528:DC%2BD1MXms1SqsL4%3D]; Bibcode number [2009SSCom.149.1072A] 10.1016/j.ssc.2009.02.041CrossRefGoogle Scholar